#------------------------------------------------------------------------------
#$Date: 2018-09-04 15:37:58 +0300 (Tue, 04 Sep 2018) $
#$Revision: 210405 $
#$URL: file:///home/coder/svn-repositories/cod/cif/7/11/37/7113714.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7113714
loop_
_publ_author_name
'Moulton, Brian'
'Abourahma, Heba'
'Bradner, Michael W.'
'Lu, Jianjiang'
'McManus, Gregory J.'
'Zaworotko, Michael J.'
_publ_section_title
;
 A new 6⁵.8 topology and a distorted 6⁵.8 CdSO₄ topology: two new
 supramolecular isomers of [M₂(bdc)₂(L)₂]ₙ coordination polymers
;
_journal_coden_ASTM              CHCOFS
_journal_issue                   12
_journal_name_full
;
 Chemical Communications (Cambridge, United Kingdom)
;
_journal_page_first              1342
_journal_page_last               1343
_journal_paper_doi               10.1039/b301221b
_journal_year                    2003
_chemical_formula_sum            'C17 H11 Co N O6.48'
_chemical_formula_weight         391.80
_space_group_IT_number           167
_symmetry_cell_setting           rhombohedral
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            36
_cell_length_a                   30.3087(15)
_cell_length_b                   30.3087(15)
_cell_length_c                   18.3364(13)
_cell_measurement_temperature    173(2)
_cell_volume                     14587.4(15)
_computing_cell_refinement       'Bruker SMART'
_computing_data_collection       'Bruker SMART'
_computing_data_reduction        'Bruker SHELXTL'
_computing_molecular_graphics    'Bruker SHELXTL'
_computing_publication_material  'Bruker SHELXTL'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.987
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0760
_diffrn_reflns_av_sigmaI/netI    0.0816
_diffrn_reflns_limit_h_max       37
_diffrn_reflns_limit_h_min       -39
_diffrn_reflns_limit_k_max       37
_diffrn_reflns_limit_k_min       -39
_diffrn_reflns_limit_l_max       24
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            30199
_diffrn_reflns_theta_full        28.27
_diffrn_reflns_theta_max         28.27
_diffrn_reflns_theta_min         1.34
_exptl_absorpt_coefficient_mu    1.096
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            red/purpl
_exptl_crystal_density_diffrn    1.606
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             7157
_exptl_crystal_size_max          0.25
_exptl_crystal_size_mid          0.75
_exptl_crystal_size_min          0.25
_refine_diff_density_max         0.654
_refine_diff_density_min         -0.407
_refine_diff_density_rms         0.120
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   0.939
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     244
_refine_ls_number_reflns         3985
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      0.939
_refine_ls_R_factor_all          0.0757
_refine_ls_R_factor_gt           0.0455
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0523P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1079
_refine_ls_wR_factor_ref         0.1153
_reflns_number_gt                2650
_reflns_number_total             3985
_reflns_threshold_expression     >2sigma(I)
_cod_duplicate_entry             7103694
_cod_data_source_file            b301221b.txt
_cod_data_source_block           mbco35
_cod_depositor_comments
;
The following automatic conversions were performed:

'_symmetry_cell_setting' value 'Rhombohedral' changed to
'rhombohedral' according to
/usr/data/users/saulius/automatic-downloads/retrospective/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26.

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 
;
_cod_original_sg_symbol_H-M      R-3c
_cod_database_code               7113714
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'y, x, -z+1/2'
'x-y, -y, -z+1/2'
'-x, -x+y, -z+1/2'
'x+2/3, y+1/3, z+1/3'
'-y+2/3, x-y+1/3, z+1/3'
'-x+y+2/3, -x+1/3, z+1/3'
'y+2/3, x+1/3, -z+5/6'
'x-y+2/3, -y+1/3, -z+5/6'
'-x+2/3, -x+y+1/3, -z+5/6'
'x+1/3, y+2/3, z+2/3'
'-y+1/3, x-y+2/3, z+2/3'
'-x+y+1/3, -x+2/3, z+2/3'
'y+1/3, x+2/3, -z+7/6'
'x-y+1/3, -y+2/3, -z+7/6'
'-x+1/3, -x+y+2/3, -z+7/6'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'-y, -x, z-1/2'
'-x+y, y, z-1/2'
'x, x-y, z-1/2'
'-x+2/3, -y+1/3, -z+1/3'
'y+2/3, -x+y+1/3, -z+1/3'
'x-y+2/3, x+1/3, -z+1/3'
'-y+2/3, -x+1/3, z-1/6'
'-x+y+2/3, y+1/3, z-1/6'
'x+2/3, x-y+1/3, z-1/6'
'-x+1/3, -y+2/3, -z+2/3'
'y+1/3, -x+y+2/3, -z+2/3'
'x-y+1/3, x+2/3, -z+2/3'
'-y+1/3, -x+2/3, z+1/6'
'-x+y+1/3, y+2/3, z+1/6'
'x+1/3, x-y+2/3, z+1/6'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Co1 Co 0.306224(16) 0.188734(16) 0.13346(2) 0.01866(13) Uani 1 1 d .
N1 N 0.26346(10) 0.20331(10) 0.05834(14) 0.0198(6) Uani 1 1 d .
O1 O 0.34929(9) 0.18989(9) 0.27857(12) 0.0275(5) Uani 1 1 d .
O2 O 0.37697(8) 0.24265(8) 0.10374(13) 0.0256(5) Uani 1 1 d .
O3 O 0.31067(9) 0.22775(9) 0.22492(12) 0.0266(5) Uani 1 1 d .
O4 O 0.41948(8) 0.20932(8) 0.15963(12) 0.0263(5) Uani 1 1 d .
C1 C 0.20185(13) 0.19841(13) 0.14589(19) 0.0270(8) Uani 1 1 d .
H1 H 0.2217 0.1964 0.1845 0.032 Uiso 1 1 calc R
C2 C 0.41711(12) 0.24335(12) 0.12336(17) 0.0212(7) Uani 1 1 d .
C3 C 0.33064(11) 0.24327(11) 0.35078(17) 0.0192(7) Uani 1 1 d .
C4 C 0.46595(14) 0.3333 0.0833 0.0188(9) Uani 1 2 d S
H4 H 0.4346 0.3333 0.0833 0.023 Uiso 1 2 calc SR
C5 C 0.21832(12) 0.20259(12) 0.07315(18) 0.0220(7) Uani 1 1 d .
C6 C 0.32914(12) 0.28872(12) 0.35164(18) 0.0228(7) Uani 1 1 d .
H6 H 0.3252 0.3026 0.3073 0.027 Uiso 1 1 calc R
C7 C 0.3333 0.22219(14) 0.4167 0.0186(9) Uani 1 2 d S
H7 H 0.3333 0.1909 0.4167 0.022 Uiso 1 2 calc SR
C8 C 0.33006(12) 0.21838(12) 0.27989(17) 0.0217(7) Uani 1 1 d .
C9 C 0.3333 0.31333(14) 0.4167 0.0255(11) Uani 1 2 d S
H9 H 0.3333 0.3447 0.4167 0.031 Uiso 1 2 calc SR
C10 C 0.46644(12) 0.28973(11) 0.10287(17) 0.0190(7) Uani 1 1 d .
C11 C 0.18877(13) 0.20658(13) 0.0163(2) 0.0274(8) Uani 1 1 d .
C12 C 0.20724(14) 0.21294(14) -0.0552(2) 0.0355(9) Uani 1 1 d .
H12 H 0.1884 0.2162 -0.0942 0.043 Uiso 1 1 calc R
C13 C 0.25190(15) 0.21451(14) -0.06880(19) 0.0341(9) Uani 1 1 d .
H13 H 0.2649 0.2192 -0.1170 0.041 Uiso 1 1 calc R
C14 C 0.27854(13) 0.20909(12) -0.01014(18) 0.0261(8) Uani 1 1 d .
H14 H 0.3095 0.2096 -0.0205 0.031 Uiso 1 1 calc R
C15 C 0.14286(13) 0.20543(14) 0.0345(2) 0.0370(9) Uani 1 1 d .
H15 H 0.1228 0.2082 -0.0031 0.044 Uiso 1 1 calc R
C16 C 0.15686(14) 0.19724(14) 0.1604(2) 0.0353(9) Uani 1 1 d .
H16 H 0.1457 0.1942 0.2095 0.042 Uiso 1 1 calc R
C17 C 0.55694(16) 0.3333 0.0833 0.0305(12) Uani 1 2 d S
H17 H 0.5883 0.3333 0.0833 0.037 Uiso 1 2 calc SR
C18 C 0.51247(12) 0.29007(12) 0.10508(19) 0.0250(8) Uani 1 1 d .
H18 H 0.5135 0.2608 0.1214 0.030 Uiso 1 1 calc R
C19 C 0.12713(14) 0.20042(15) 0.1047(2) 0.0393(10) Uani 1 1 d .
H19 H 0.0959 0.1991 0.1160 0.047 Uiso 1 1 calc R
O101 O 0.2861(8) 0.5838(6) 0.2002(10) 0.119(5) Uiso 0.38 1 d P
O102 O 0.3342(5) 0.6087(6) 0.0090(8) 0.118(4) Uiso 0.38 1 d P
O103 O 0.3333 0.6667 -0.0205(17) 0.122(10) Uiso 0.30 3 d SP
O104 O 0.3370(7) 0.5993(7) 0.0814(11) 0.154(6) Uiso 0.38 1 d P
O105 O 0.2539(13) 0.5889(13) 0.149(2) 0.188(11) Uiso 0.25 1 d P
O106 O 0.2927(9) 0.5872(7) 0.1258(12) 0.106(6) Uiso 0.25 1 d P
O107 O 0.2983(9) 0.6474(11) 0.0232(15) 0.169(11) Uiso 0.25 1 d P
O108 O 0.2858(9) 0.6216(9) 0.0983(13) 0.128(7) Uiso 0.25 1 d P
O109 O 0.2545(11) 0.5584(11) 0.2181(16) 0.156(10) Uiso 0.25 1 d P
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0033 0.0016 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0061 0.0033 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Co Co 0.3494 0.9721 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Co1 O3 90.99(10) . .
O2 Co1 O4 162.29(9) . 25
O3 Co1 O4 91.87(9) . 25
O2 Co1 N1 99.88(10) . .
O3 Co1 N1 106.94(10) . .
O4 Co1 N1 95.99(10) 25 .
O2 Co1 O1 83.81(9) . 25
O3 Co1 O1 162.66(9) . 25
O4 Co1 O1 88.33(9) 25 25
N1 Co1 O1 90.27(9) . 25
O2 Co1 Co1 82.37(7) . 25
O3 Co1 Co1 91.99(7) . 25
O4 Co1 Co1 80.07(7) 25 25
N1 Co1 Co1 160.84(8) . 25
O1 Co1 Co1 70.96(6) 25 25
C14 N1 C5 117.6(3) . .
C14 N1 Co1 116.5(2) . .
C5 N1 Co1 125.5(2) . .
C8 O1 Co1 136.9(2) . 25
C2 O2 Co1 124.3(2) . .
C8 O3 Co1 115.6(2) . .
C2 O4 Co1 127.0(2) . 25
C16 C1 C5 119.3(3) . .
O2 C2 O4 126.0(3) . .
O2 C2 C10 116.5(3) . .
O4 C2 C10 117.5(3) . .
C7 C3 C6 118.7(3) . .
C7 C3 C8 120.8(3) . .
C6 C3 C8 120.5(3) . .
C10 C4 C10 121.2(4) . 17_554
N1 C5 C1 119.4(3) . .
N1 C5 C11 121.1(3) . .
C1 C5 C11 119.5(3) . .
C9 C6 C3 120.2(3) . .
C3 C7 C3 121.4(4) . 12
O1 C8 O3 124.3(3) . .
O1 C8 C3 117.9(3) . .
O3 C8 C3 117.8(3) . .
C6 C9 C6 120.6(4) 12 .
C4 C10 C18 119.5(3) . .
C4 C10 C2 118.7(3) . .
C18 C10 C2 121.7(3) . .
C12 C11 C15 123.0(3) . .
C12 C11 C5 118.3(3) . .
C15 C11 C5 118.7(3) . .
C13 C12 C11 120.0(3) . .
C12 C13 C14 118.6(3) . .
N1 C14 C13 124.4(3) . .
C19 C15 C11 120.9(3) . .
C1 C16 C19 121.6(4) . .
C18 C17 C18 120.2(4) 17_554 .
C17 C18 C10 119.7(3) . .
C15 C19 C16 120.0(3) . .
O109 O101 O104 62(2) . 26_455
O109 O101 O105 136(3) . 27
O104 O101 O105 138(3) 26_455 27
O109 O101 O106 117(3) . .
O104 O101 O106 142(2) 26_455 .
O105 O101 O106 71.5(17) 27 .
O109 O101 O108 132(3) . 27
O104 O101 O108 82.0(17) 26_455 27
O105 O101 O108 58.4(18) 27 27
O106 O101 O108 110.3(19) . 27
O109 O101 O105 81(3) . .
O104 O101 O105 90.8(19) 26_455 .
O105 O101 O105 125.3(19) 27 .
O106 O101 O105 54.1(15) . .
O108 O101 O105 133(2) 27 .
O107 O102 O104 88.0(19) 2_665 .
O107 O103 O107 82(3) . 3_565
O107 O103 O107 82(3) . 2_665
O107 O103 O107 82(3) 3_565 2_665
O109 O104 O101 44.9(16) 27 27
O109 O104 O102 134(2) 27 .
O101 O104 O102 137.3(19) 27 .
O109 O104 O106 107(2) 27 .
O101 O104 O106 95.1(17) 27 .
O102 O104 O106 116.7(19) . .
O109 O104 O108 92(2) 27 2_665
O101 O104 O108 52.0(13) 27 2_665
O102 O104 O108 91.3(15) . 2_665
O106 O104 O108 103.8(14) . 2_665
O109 O104 O107 131(2) 27 2_665
O101 O104 O107 103.0(18) 27 2_665
O102 O104 O107 40.6(12) . 2_665
O106 O104 O107 111.8(17) . 2_665
O108 O104 O107 52.0(12) 2_665 2_665
O106 O105 O108 57.9(19) . .
O106 O105 O101 118(3) . 26_455
O108 O105 O101 62(2) . 26_455
O106 O105 O101 61.0(17) . .
O108 O105 O101 105(3) . .
O101 O105 O101 128(3) 26_455 .
O106 O105 O109 88(3) . .
O108 O105 O109 140(3) . .
O101 O105 O109 138(3) 26_455 .
O101 O105 O109 35.9(15) . .
O106 O105 O106 126(3) . 26_455
O108 O105 O106 101(2) . 26_455
O101 O105 O106 54.6(14) 26_455 26_455
O101 O105 O106 83(2) . 26_455
O109 O105 O106 84(2) . 26_455
O108 O106 O105 64(2) . .
O108 O106 O101 112(2) . .
O105 O106 O101 64.9(19) . .
O108 O106 O104 95(2) . .
O105 O106 O104 158(3) . .
O101 O106 O104 131(2) . .
O108 O106 O105 134(2) . 27
O105 O106 O105 118.4(18) . 27
O101 O106 O105 53.8(14) . 27
O104 O106 O105 77.9(19) . 27
O102 O107 O103 103(3) 3_565 .
O102 O107 O108 114(3) 3_565 .
O103 O107 O108 140(3) . .
O102 O107 O107 91(3) 3_565 3_565
O103 O107 O107 49.2(13) . 3_565
O108 O107 O107 113.0(12) . 3_565
O102 O107 O107 148(3) 3_565 2_665
O103 O107 O107 49.2(13) . 2_665
O108 O107 O107 91(2) . 2_665
O107 O107 O107 60.000(11) 3_565 2_665
O102 O107 O104 51.4(15) 3_565 3_565
O103 O107 O104 141(3) . 3_565
O108 O107 O104 64.0(16) . 3_565
O107 O107 O104 98(2) 3_565 3_565
O107 O107 O104 138.0(12) 2_665 3_565
O106 O108 O105 58.3(19) . .
O106 O108 O101 117(2) . 26_455
O105 O108 O101 59.7(18) . 26_455
O106 O108 O107 133(3) . .
O105 O108 O107 153(3) . .
O101 O108 O107 109(2) 26_455 .
O106 O108 O104 163(2) . 3_565
O105 O108 O104 104(2) . 3_565
O101 O108 O104 46.0(12) 26_455 3_565
O107 O108 O104 64.0(16) . 3_565
O101 O109 O104 73(2) . 26_455
O101 O109 O105 63(2) . .
O104 O109 O105 87(2) 26_455 .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Co1 O2 2.015(2) .
Co1 O3 2.017(2) .
Co1 O4 2.021(2) 25
Co1 N1 2.085(3) .
Co1 O1 2.132(2) 25
Co1 Co1 2.8584(8) 25
N1 C14 1.318(4) .
N1 C5 1.384(4) .
O1 C8 1.261(4) .
O1 Co1 2.132(2) 25
O2 C2 1.259(4) .
O3 C8 1.269(4) .
O4 C2 1.259(4) .
O4 Co1 2.021(2) 25
C1 C16 1.372(5) .
C1 C5 1.408(5) .
C2 C10 1.500(4) .
C3 C7 1.388(4) .
C3 C6 1.401(4) .
C3 C8 1.499(4) .
C4 C10 1.377(4) .
C4 C10 1.377(4) 17_554
C5 C11 1.418(5) .
C6 C9 1.378(4) .
C7 C3 1.388(4) 12
C9 C6 1.378(4) 12
C10 C18 1.391(4) .
C11 C12 1.401(5) .
C11 C15 1.414(5) .
C12 C13 1.354(5) .
C13 C14 1.403(5) .
C15 C19 1.354(5) .
C16 C19 1.397(5) .
C17 C18 1.388(4) 17_554
C17 C18 1.388(4) .
O101 O109 0.94(3) .
O101 O104 1.27(2) 26_455
O101 O105 1.36(3) 27
O101 O106 1.38(2) .
O101 O108 1.39(2) 27
O101 O105 1.42(3) .
O102 O107 1.14(3) 2_665
O102 O104 1.37(2) .
O103 O107 1.22(3) .
O103 O107 1.22(3) 3_565
O103 O107 1.22(3) 2_665
O104 O109 1.18(3) 27
O104 O101 1.27(2) 27
O104 O106 1.45(2) .
O104 O108 1.75(3) 2_665
O104 O107 1.75(3) 2_665
O105 O106 1.27(3) .
O105 O108 1.34(4) .
O105 O101 1.36(3) 26_455
O105 O109 1.58(4) .
O105 O106 1.60(3) 26_455
O106 O108 1.27(3) .
O106 O105 1.60(3) 27
O107 O102 1.14(3) 3_565
O107 O108 1.53(3) .
O107 O107 1.60(4) 3_565
O107 O107 1.60(4) 2_665
O107 O104 1.75(3) 3_565
O108 O101 1.39(2) 26_455
O108 O104 1.75(3) 3_565
O109 O104 1.18(3) 26_455
